a prediction method for in-plane permeability and ... measuring permeability, but permeability...
Post on 14-Mar-2020
Embed Size (px)
Engineering, 2011, 3, 691-699 doi:10.4236/eng.2011.37082 Published Online July 2011 (http://www.SciRP.org/journal/eng)
Copyright © 2011 SciRes. ENG
A Prediction Method for in-Plane Permeability and Manufacturing Applications in the VARTM Process
Ya-Jung Lee1*, Yu-Ti Jhan1, Cheng-Hsien Chung2, Yao Hsu3 1Engineering Science and Ocean Engineering, National Taiwan University, Chinese Taipei
2R&D Department, United Ship Design & Development Center, Taipei 3Business and Entrepreneurial Management, Kai Nan University, Taoyuan, Chinese Taipei
E-mail: *email@example.com Received April 15, 2011; revised May 3, 2011; accepted May 20, 2011
Abstract VARTM (Vacuum Assisted Resin Transfer Molding) is a popular method for manufacturing large-scaled, single-sided mold composite structures, such as wind turbine blades and yachts. Simulation to find the proper infusion scenario before manufacturing is essential to avoid dry spots as well as incomplete saturation and various fiber weaves with different permeability affect numerical simulation tremendously. This study fo- cused on deriving the in-plane permeability prediction method for FRP (Fiber Reinforced Plastics) laminates in the VARTM process by experimental measurements and numerical analysis. The method provided an ef- ficient way to determine the permeability of laminates without conducting lots of experiments in the future. In-plane permeability imported into the software, RTM-Worx, to simulate resin flowing pattern before the infusion experiments of a 3D ship hull with two different infusion scenarios. The close agreement between experiments and simulations proved the correctness and applicability of the prediction method for the in-plane permeability. Keywords: Prediction Method, in-Plane Permeability, Manufacturing Simulation, Infusion Scenarios
1. Introduction VARTM (Vacuum Assisted Rein Transfer Molding) has been employed successfully to manufacture FRP (Fiber Reinforced Plastics) ship hull structures since 1994  and other large structures, such as wind turbine blades and yachts [2-3]. In this manufacturing technique, the fiber lay-up is placed in advance above a one-sided mold, and resin injects into the fiber lay-up under one pressure gradient as vacuum is applied. This procedure provides the advantages of low VOC (Volatile Organic Com- pounds) emission as well as stable and excellent me- chanical properties of products. The manufacturing fail- ure risks, such as void contain and incomplete saturation, increase as the structure dimension increases. Accord- ingly, resin flowing prediction before manufacturing complex structures with various fiber laminates is essen- tial. The CV-FEM (control volume finite element method) is utilized to explicate the behavior of resin flowing in fiber laminates [4,5]. With respect to the VARTM simulation, Mohan  modeled flow in chan-
nels based on a finite element method. Sun  and Ni  applied CV-FEM to predict the filling time and pattern associated with high-permeable medium and grooves in the SCRIMP process. Koorevaar [9,10] adopted 2.5D flow models, meaning that resin flow in the thickness direction is neglected, although the geometries are de- scribed as 3D, to simulate the VARTM and RTM proc- ess. The VARTM simulation involves with parameters, such as the viscosity of resin, the porosity and perme- ability of fiber laminates. The permeability of FRP laminates is critical in the manufacturing process and numerous researchers have investigated the measure- ments and analytical models of permeability [7,8] [11-15]. Sun  and Ni  set up a device to visualize the experimental results and measurements of permeabil- ity. Wang and Demaria [11-13] characterized the in-plane permeability of woven fabrics and proposed a predictive model. Wu  and Nedanov  researched the trans-plane permeability by theory and experiments to describe 3D permeability of fiber laminates. Some researchers have described the flow using equivalent
Y.-J. LEE ET AL.
Copyright © 2011 SciRes. ENG
permeability [16-18]. For example, Dong  increased the thickness of the distribution medium and/or the fiber preform to obtain equivalent material permeability. Be- sides, the Kozeny-Carman equation was commonly util- ized to discuss the flow impregnates inside the porous material when considering the dimension of fiber [19-22]. Gebart  investigated the permeability of an idealized unidirectional reinforcement through the Darcy’s law and Kozeny-Carman equation, and Rahatekar  used the permeability models through Kozeny-Carman equa- tion to discuss the relationship between injection pultru- sion pressure and process control parameters.
The infusion scenario in the VARTM process includ- ing the numbers of flowing channels, injection and vent- ing ports, and the triggering timing of the injection gates etc. determines the impregnation of FRP products. Pre- cise evaluation of the resin flowing pattern before fabri- cation reduces the risk and cost of manufacturing failure. Therefore, some researchers [23,24] focused on how to arrange and improve the infusion process to avoid dry spots and incompletely saturation. Han  and Kang  analyzed the VARTM process under different vac- uum conditions as well as infusion strategy and simu- lated the infusion process of a boat hull. The above- mentioned studies have provided feasible methods for measuring permeability, but permeability measurement through the experiments is a time-consuming procedure. Hence, the development of simplified macroscopic mod- els for predicting permeability of FRP laminates com- posing of various woven fabrics is beneficial for simu- lating and discussing the manufactures of complex structures with various infusion scenarios in the VARTM process. This study investigated the in-plane permeabil- ity for single and multi types of fiber laminates by the permeability experiments. A prediction method for the in-plane permeability was established by defining the parameter of “thickness porosity”, and the method pro- vided an efficient way to determine the in-plane perme- ability of FRP laminates without conducting time-con- suming experiments. Flowing patterns of a 3D ship hull with two different infusion scenarios were simulated to compare with the manufacturing experiments. The close agreement between experiments and simulations proved the correctness and applicability of the prediction method for the in-plane permeability. 2. In-Plane Permeability Experiments Experimental Measurements and Discussion
Several scholars have utilized Equation (1), derived from Darcy’s Law, to describe the resin flowing process inside the porous space of fabrics under the RTM or VARTM method from 1980 to date.
1 xx xy xz yx yy yz
zx zy zz
P xu K K K Pv K K K y
w K K K P z
where V represents the Darcian Velocity, K is the tensor of permeability, μ is the viscosity of resin, and P is the gradient of pressure. In the research, realizing the in-plane permeant characteristic of FRP laminates was the main objective, and the length and width scale of fiber laminates was relatively larger than its thickness. Hence, the governing Equation (1) transformed into a 1D flowing Equation (2) when operating the rectangle ex- perimental arrangement.
2 K L
where P is the pressure gradient, is the porosity of laminate, L is the flow front, and t is the infusion time. Equation (2) reveals that the combination of value L2/t, evaluating from the video records of flowing processes, the porosity of fiber laminates, and resin viscosity de- rives the in-plane permeability (K).
The viscosity of polyester resin, μ, changing with temperature (Figure 1(a)) was measured by the Brook- field viscometer and the thermostat sink (Figure 1(b)). The infusion time of the experimental process did not exceed 30 minutes and the ambient temperature did not change sharply during the infusion time. Accordingly, the viscosity was reasonably regarded as constant throughout the whole process. Figure 2(a) displays the in-plane permeability experimental schema. The fiber assembly was rectangular, and the dimensions of fiber laminates were 48 cm × 16 cm. Pressure gradient de- signed to be along the length of fiber laminates, from injection gate to venting port. The extensible spring linking with the injection gate was placed in the starting position to transform a point-injection into a line-injec- tion, and consequently resin flowing front was perpen- dicular to the infusion direction (Figure 2(b)). Table 1 presents the single-type fiber laminates under considera- tion, including strand chopped mat, woven roving and axial fabrics with different area density and numbers of layers. Figure 3 shows the relationship between flowing fronts and its consuming infusion time which determines the permeability of FRP laminates. Initial time-delay region on the bottom surface was neglected due to the transverse-plane infusion from top surface to bottom
Y.-J. LEE ET AL.
Copyright © 2011 SciRes.